DOI: 10.17188/1294744
title: Materials Data on Li2VFe(P2O7)2 by Materials Project

description: Li2VFe(P2O7)2 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are six inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.09 Å. In the second Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 2.00–2.08 Å. In the third Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 2.00–2.08 Å. In the fourth Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 2.00–2.09 Å. In the fifth Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.08 Å. In the sixth Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 2.00–2.09 Å. There are three inequivalent V3+ sites. In the first V3+ site, V3+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.99–2.07 Å. In the second V3+ site, V3+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.99–2.08 Å. In the third V3+ site, V3+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 2.00–2.08 Å. There are three inequivalent Fe3+ sites. In the first Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Fe–O bond distances ranging from 1.97–2.09 Å. In the second Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Fe–O bond distances ranging from 1.97–2.08 Å. In the third Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Fe–O bond distances ranging from 1.97–2.09 Å. There are twelve inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two FeO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 45–49°. There are a spread of P–O bond distances ranging from 1.53–1.61 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two FeO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–49°. There are a spread of P–O bond distances ranging from 1.52–1.63 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 34–48°. There are a spread of P–O bond distances ranging from 1.52–1.63 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 45–49°. There are a spread of P–O bond distances ranging from 1.53–1.62 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–48°. There are a spread of P–O bond distances ranging from 1.52–1.63 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 45–50°. There are a spread of P–O bond distances ranging from 1.53–1.61 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 45–49°. There are a spread of P–O bond distances ranging from 1.53–1.62 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 34–50°. There are a spread of P–O bond distances ranging from 1.52–1.63 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two FeO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 45–49°. There is three shorter (1.53 Å) and one longer (1.62 Å) P–O bond length. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two FeO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–48°. There are a spread of P–O bond distances ranging from 1.52–1.63 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two FeO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 34–50°. There are a spread of P–O bond distances ranging from 1.52–1.63 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two FeO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 45–49°. There are a spread of P–O bond distances ranging from 1.53–1.61 Å. There are forty-two inequivalent O2- sites. In the first O2- site, O2- is bonded in a bent 150 degrees geometry to one Fe3+ and one P5+ atom. In the second O2- site, O2- is bonded in a distorted T-shaped geometry to one Li1+, one Fe3+, and one P5+ atom. In the third O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one V3+ and one P5+ atom. In the fourth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Fe3+, and one P5+ atom. In the fifth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Fe3+, and one P5+ atom. In the sixth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Fe3+, and one P5+ atom. In the seventh O2- site, O2- is bonded in a 2-coordinate geometry to one Fe3+ and one P5+ atom. In the eighth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the ninth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the tenth O2- site, O2- is bonded in a distorted T-shaped geometry to one Li1+, one V3+, and one P5+ atom. In the eleventh O2- site, O2- is bonded in a bent 150 degrees geometry to one V3+ and one P5+ atom. In the twelfth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V3+, and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V3+, and one P5+ atom. In the fourteenth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V3+, and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V3+ and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a distorted T-shaped geometry to one Li1+, one V3+, and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the eighteenth O2- site, O2- is bonded in a 2-coordinate geometry to one Fe3+ and one P5+ atom. In the nineteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Fe3+, and one P5+ atom. In the twentieth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V3+, and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V3+, and one P5+ atom. In the twenty-second O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Fe3+, and one P5+ atom. In the twenty-third O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V3+, and one P5+ atom. In the twenty-fourth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V3+, and one P5+ atom. In the twenty-fifth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one V3+ and one P5+ atom. In the twenty-sixth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the twenty-seventh O2- site, O2- is bonded in a distorted T-shaped geometry to one Li1+, one Fe3+, and one P5+ atom. In the twenty-eighth O2- site, O2- is bonded in a bent 150 degrees geometry to one Fe3+ and one P5+ atom. In the twenty-ninth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Fe3+, and one P5+ atom. In the thirtieth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V3+, and one P5+ atom. In the thirty-first O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V3+, and one P5+ atom. In the thirty-second O2- site, O2- is bonded in a bent 150 degrees geometry to one V3+ and one P5+ atom. In the thirty-third O2- site, O2- is bonded in a distorted T-shaped geometry to one Li1+, one V3+, and one P5+ atom. In the thirty-fourth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the thirty-fifth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the thirty-sixth O2- site, O2- is bonded in a 2-coordinate geometry to one Fe3+ and one P5+ atom. In the thirty-seventh O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Fe3+, and one P5+ atom. In the thirty-eighth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Fe3+, and one P5+ atom. In the thirty-ninth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Fe3+, and one P5+ atom. In the fortieth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one V3+ and one P5+ atom. In the forty-first O2- site, O2- is bonded in a distorted T-shaped geometry to one Li1+, one Fe3+, and one P5+ atom. In the forty-second O2- site, O2- is bonded in a bent 150 degrees geometry to one Fe3+ and one P5+ atom.